International Journal of ElectrochemistryVolume 2012 (2012), Article ID 758708, 5 pagesdoi:10.1155/2012/758708

Research Article

Anodic Stripping Voltammetry of Se⁴⁺ on Gold-Modified Boron-Doped Diamond Electrodes

Stéphane Fierro,¹ Takeshi Watanabe,¹ Kazumi Akai,¹ Mikito Yamanuki,² and Yasuaki Einaga1,3

¹Department of Chemistry, Faculty of Science and Technology, Keio University, 3-14-1 Hiyoshi, Yokohama 223-8522, Japan²Advancec R&D Center, HORIBA Ltd., Minami-ku, Kyoto 601-8510, Japan³JST, CREST, 3-14-1 Hiyoshi, Yokohama 223-8522, Japan

Received 6 April 2011; Accepted 22 May 2011

Academic Editor: Giancarlo R. Salazar-Banda

Copyright © 2012 Stéphane Fierro et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Electrochemical detection of Se⁴⁺ has been performed by anodic stripping voltammetry on a boron-doped diamond (BDD) electrode modified with gold nanoparticles deposited through chronocoulometry. This method is based on the affinity between the gold nanoparticles and Se⁰, while the BDD electrode is presented as an ideal material for metal modification due to its unique properties. The resulting anodic stripping voltammograms exhibited a clear peak at 0.9 V versus AgCl related to Se⁴⁺, and highly accurate () calibration curves could be obtained for a selenium concentration range between 10 and 100 μg/L. The influence of Se deposition time and other metals dissolved in solution (Cu, Cd, Pb, Cr, and B) has been investigated as well, and it was found that the Se⁴⁺ calibration curves remained unaltered. For all the experiments performed, a detection limit around 10 μg/L was achieved. The high accuracy and reproducibility of the results as well as the excellent stability of the electrode material proves the excellent capabilities of this system for selenium detection.

1. Introduction

Selenium is an essential micronutrient for animals and humans but can be extremely toxic if absorbed in large doses (over 400 μg per day) [1]. Exceeding the tolerable upper intake level of 400 micrograms per day (15 μg per kg bodyweight) can lead to selenosis, which affects the respiratory, digestive, and neurological systems [2]. The maximum contaminant level of selenium in water allowed by the US Environmental Protection Agency is 50 μg/L [3].

Selenium exists in many forms in the environment, but the most abundant are H₂SeO₃ (Se⁴⁺), H₂SeO₄ (Se⁶⁺), and their derivatives [4]. The quantification of both forms is important because Se species vary in their toxicity potential to animals and humans. However, if one sample contains both Se⁴⁺ and Se⁶⁺ species, it is possible to reduce the Se⁶⁺ to Se⁴⁺ by heating the sample at 85°C in concentrated HCl [4]. The concentration of Se in this solution is then considered as the sum of Se⁴⁺ and Se⁶⁺. The difference between the concentration of Se in digested and undigested samples is the concentration of Se⁶⁺. Many techniques have been developed in order to analyze Se⁴⁺ concentrations at the μg/L level but the most common method is stripping voltammetry due to its simplicity, rapidity, and excellent sensitivity. Both cathodic stripping voltammetry using a hanging mercury drop electrode [5–11] and anodic stripping voltammetry (ASV) using gold (rotating disk or film) electrodes [12–14] have been extensively studied for Se⁴⁺ determination in acidic solutions. These methods have been shown to be quite efficient for selenium determination. However, the anodic stripping on gold electrodes usually requires time-consuming pretreatments of the gold electrode in order to get reproducible results. Moreover, the main problem of these methods is the splitting of the stripping peaks [5, 6]. Several methods have been proposed to solve this problem like increasing the temperature of the support electrolyte [6, 8] or adding small amounts of copper or rhodium to the solutions [7–9, 11, 15]. Nevertheless, these steps tend to complicate the experimental procedure, and added to the delicate handling of mercury electrodes, these methods become less suited for real analytical applications.

In this work, the detection of Se⁴⁺ by anodic stripping voltammetry on gold-modified boron-doped diamond electrode is presented for the first time. BDD has been selected for gold deposition due to its outstanding properties compared to other conventional electrode materials such as a wide electrochemical potential window, low background current, and weak adsorption of polar molecules [16, 17]. These properties offer a significant advantage for metal modification as it was already shown for the detection of As³⁺ and As⁵⁺ mixtures [18]. Moreover, the high stability of these gold-modified BDD electrodes has been shown [18]. Therefore, the same method has been used for selenium detection in this study. Concentration of Se⁴⁺ was measured by a stripping method based on the simple electrochemical reduction of Se⁴⁺ to Se⁰ followed by oxidation of the latter. The influence of Se deposition time is discussed. Moreover, the selective detection of Se⁴⁺ in the presence of interference metal ions was also studied.

2. Experimental

2.1. Chemicals and Materials

Selenious acid (H₂SeO₃), hydrogen tetrachloroaurate(III)trihydrate (HAuCl₄), hydrogen chloride (HCl), perchloric acid (HClO₄), copper chloride (CuCl₂), lead chloride (PbCl₂), boric acid (H₃BO₃), cadmium chloride (CdCl₂), and potassium dichromate (K₂Cr₂O₇) were purchased from Wako. All chemicals were used without further purification.

2.2. Preparation of BDD Electrodes

BDD thin films were deposited using a microwave plasma-assisted chemical vapor deposition (MPCVD) setup (ASTeX Corp.). Acetone was used as carbon source and B(OCH₃)₃ as boron source. The concentration of the latter was 0.1% w/w in source. The surface morphology and crystalline structures were characterized using scanning electron microscopy (not shown in this work). The typical size of the diamond crystals was about 5 μm. BDD films were deposited on Si (1 0 0) wafers in the MPCVD chamber at 5 kW using high-purity hydrogen as carrier gas. The BDD film thickness was about 40 μm after 10 hours of deposition. The Raman spectrum of this film exhibited a sharp peak at 1334 cm⁻¹, which is characteristic of crystalline diamond. The BDD electrodes were pretreated by ultrasonication in 2-propanol for about 10 minutes followed by rinsing with high-purity water in order to remove any organic impurities that may have remained within the BDD film after deposition in the MPCVD chamber.

Gold-modified BDD electrodes were prepared through the same procedure reported in [19]. The BDD electrode was immersed in 0.1 M HCl solution containing 100 ppm of HAuCl₄, and gold nanoparticles deposition was performed through chronocoulometry.

2.3. Electrochemical Measurements

Electrochemical measurements were carried out in a single-compartment cell using a Hokuto Denko Hz-5000 potentiostat at room temperature (23°C). The reference electrode was Ag/AgCl, the counter electrode was a platinum wire, and the working electrode was BDD. The working geometric area was 0.283 cm². The anodic stripping of Se was performed in 0.1 M HClO₄, whereas the posttreatment was carried out in 0.1 M HCl. In this work, all potentials given are with respect to the Ag/AgCl reference electrode (0.2 V versus SHE).

3. Results and Discussion

3.1. Anodic Stripping Voltammetry of Se⁴⁺

The anodic stripping voltammetry of Se⁴⁺ has been performed based on its reduction to Se⁰ followed by oxidation of the latter. For the first measurements, gold particles were deposited through chronocoulometry at −35 mC cm⁻² for 1 minute. A deposition potential of −0.4 V has been applied during 2 minutes for Se deposition because the Se⁴⁺ reduction peak was observed around that potential on gold-modified BDD electrodes (result not shown). For the stripping of selenium, the voltammetric scan was performed between the deposition potential (−0.4 V) and different upper limit potentials. The resulting voltammograms related to solutions containing different concentrations of Se⁴⁺ (from 10 to 100 μg/L dissolved in 0.1 M HClO₄) are displayed in Figure 1 for upper limit potential of 1.2 V. When the upper limit potential was fixed at 1.4 V, almost the same voltammogram as Figure 1 was observed (not shown). Both figures show the presence of a clear stripping peak situated at 0.9 V approximately, which is related to selenium. Therefore, an upper potential limit of 1.2 V was selected for the anodic stripping voltammetry measurements. The peak currents obtained from Figure 1 were therefore plotted as a function of Se⁴⁺ concentration, and the resulting graph (presented in Figure 2) shows that a linear and highly accurate calibration curve () could be obtained under these conditions for a Se⁴⁺ concentration range between 10 and 100 μg/L.

Figure 1: Stripping voltammograms of Se⁴⁺ in 0.1 M HClO₄ in the concentration range of 0–100 μg/L recorded on a BDD electrode, which was previously modified by gold nanoparticles deposited by chronocoulometry (−35 mC cm⁻² was applied for 1 minute in a solution of HAuCl₄ 100 ppm in 0.1 M HCl). The deposition potential (−0.4 V versus Ag/AgCl) was applied during 2 minutes before the stripping, which was performed at a scan rate of 200 mV/s. The upper potential limit was fixed at 1.2 V versus Ag/AgCl. °C.

Figure 2: Calibration curve from the anodic stripping voltammograms presented in Figure 1. The peak current was plotted as a function of Se⁴⁺ concentration.

One set of measurements was performed on a gold-modified electrode where the chronocoulometry was performed at −70 mC cm⁻² for 1 minute, and the resulting anodic stripping voltammograms presented on Figure 3 exhibit a similar profile; therefore, the charge applied during the modification of the BDD electrode was fixed at −35 mC cm⁻².

Figure 3: Stripping voltammograms of Se⁴⁺ in 0.1 M HClO₄ in the concentration range of 0–100 μg/L recorded on a BDD electrode, which was previously modified by gold nanoparticles deposited by chronocoulometry (−70 mC cm⁻² was applied for 1 minute in a solution of HAuCl₄ 100 ppm in 0.1 M HCl). The deposition potential (−0.4 V versus Ag/AgCl) was applied during 2 minutes before the stripping, which was performed at a scan rate of 200 mV/s. The upper potential limit was fixed at 1.2 V versus Ag/AgCl. °C.

The influence of selenium deposition time was also studied. In fact, it was reduced from 2 to 1 minute. The resulting voltammograms together with the corresponding calibration curve are displayed on Figures 4(a) and 4(b), respectively. These results show that the time during which the deposition potential is applied has no influence neither on the profile of the stripping voltammograms nor on the accuracy of the corresponding calibration curve.

(a)

(b)

Figure 4: (a) Stripping voltammograms of Se⁴⁺ in 0.1 M HClO₄ in the concentration range of 0–100 μg/L recorded on a BDD electrode, which was previously modified by gold nanoparticles deposited by chronocoulometry (−35 mC cm⁻² was applied for 1 minute in a solution of HAuCl₄ 100 ppm in 0.1 M HCl). The deposition potential (−0.4 V versus Ag/AgCl) was applied for 1 minute before the stripping, which was performed at a scan rate of 200 mV/s. The upper potential limit was fixed at 1.2 V versus Ag/AgCl. (b) Calibration curve extracted from these stripping voltammograms. °C.

3.2. Influence of Other Metal Ions

In order to evaluate the influence of other metal ions present in the media, a mixture containing cadmium, copper, boron, chromium, and lead (all at a concentration of 100 μg/L) was prepared. Anodic stripping voltammetry measurements were carried out using the aforementioned mixture and under the same conditions as those presented on Figure 1, that is, the BDD electrode was modified through chronocoulometry at −35 mC cm⁻² for 1 min in a solution of HAuCl₄ 100 mg/L in 0.1 M HCl. The deposition potential (−0.4 V) was applied during 2 minutes before performing the stripping voltammetry at 200 mV s⁻¹ between −0.4 and 1.2 V. The corresponding anodic stripping voltammograms are presented in Figure 5(a). This figure shows a clear peak at 0.9 V corresponding to selenium stripping and another peak at 0.3 V which was attributed to the stripping of copper based on measurements performed with each of the interfering metals individually (results not shown). The peaks corresponding to the stripping of the other metals (Cr, Cd, B, and Pb) have a low intensity and are located between ‒0.2 and 0 V. Nevertheless, Figure 5(a) shows clearly that selenium has the highest affinity with the gold-modified BDD electrode because the intensity of the corresponding stripping peak is the highest when concentration of the interfering metals (100 μg/L) is equal to the concentration of selenium.

(a)

(b)

Figure 5: (a) Stripping voltammograms of Se⁴⁺ (concentration range 0–100 μg/L) in CuCl₂, PbCl₂, H₃BO₃, CdCl₂, and K₂Cr₂O₇, all 100 μg/L in 0.1 M HClO₄ recorded on a BDD electrode, which was previously modified by gold nanoparticles deposited by chronocoulometry (−35 mC cm⁻² was applied for 1 minute in a solution of HAuCl₄ 100 ppm in 0.1 M HCl). The deposition potential (−0.4V versus Ag/AgCl) was applied for 2 minutes before the stripping, which was performed at a scan rate of 200 mV/s. The upper potential limit was fixed at 1.2 V versus Ag/AgCl. (b) Calibration curve extracted from these stripping voltammograms. °C.

The intensity of the anodic stripping peak of selenium was then plotted as a function of its concentration. The result, presented in Figure 5(b), shows clearly that the selenium calibration curve is still linear and accurate () despite the presence of many other interfering metals in solution.

4. Conclusions

In this study, the determination of Se⁴⁺ has been performed through anodic stripping voltammetry on boron-doped diamond electrode modified by gold particles deposited by chronocoulometry. The results have shown that a clear peak related to selenium stripping can be observed at 0.9 V and that highly accurate concentration curve could be constructed for a selenium concentration range between 10 and 100 μg/L. The influences of selenium deposition time and gold particles deposition conditions were investigated, and it was found that the accuracy of the calibration curve remained unaltered. The influence of other metal ions in solution was also studied, and the results have shown that selenium has the highest affinity with the type of electrode used herein, and accurate calibration curves for Se⁴⁺ detection could still be constructed under these conditions. These results prove that the BDD electrode modified by gold particles is an efficient material for Se⁴⁺ determination.

Acknowledgments

S. Fierro gratefully thanks the Fond National Suisse pour la Recherche Scientifique (FNSRS) for the financial support. This work was supported by New Energy and Industrial Technology Development Organization (NEDO).

References

Institute of medicine of the national academies (IOM), Dietary Reference Intake for Vitamin C, Vitamin E, Selenium, and Carotenoids, National Academy Press, Washington, DC, USA, 2000.

U. Tinggi, “Selenium toxicity and its adverse health effects,” Reviews in Food and Nutrition Toxicity, vol. 4, pp. 29–55, 2005.

US Environmental Protection Agency, http://water.epa.gov/drink/contaminants/basicinformation/selenium.cfm

K. J. Reddy, Z. Zhang, M. J. Blaylock, and G. F. Vance, “Method for detecting selenium speciation in groundwater,” Environmental Science and Technology, vol. 29, no. 7, pp. 1754–1759, 1995.

G. Jarzabek and Z. Kublik, “Cyclic and stripping voltammetry of Se(+4) and Se(-2) at the HMDE in acidic media,” Journal of Electroanalytical Chemistry, vol. 137, no. 2, pp. 247–259, 1982.

G. Jarzabek and Z. Kublik, “Determination of traces of selenium(IV) by cathodic stripping voltammetry at the hanging mercury drop electrode,” Analytica Chimica Acta, vol. 143, pp. 121–130, 1982.

S. B. Adeloju, A. M. Bond, and H. C. Hughes, “Determination of selenium, copper, lead and cadmium in biological materials by differential pulse stripping voltammetry,” Analytica Chimica Acta, vol. 148, pp. 59–69, 1983.

L. Campanella and T. Ferri, “Voltammetric behaviour of selenium(IV) at hanging mercury drop electrodes in acetate buffer,” Journal of Electroanalytical Chemistry, vol. 165, no. 1-2, pp. 241–249, 1984.

U. Baltensperger and J. Hertz, “Parameter evaluation for the determination of selenium by cathodic stripping voltammetry at the hanging mercury drop electrode,” Analytica Chimica Acta, vol. 172, pp. 49–56, 1985.

G. Mattsson, L. Nyholm, and Å. Olin, “Cathodic stripping voltammetry of Cu2Se at mercury electrodes,” Journal of Electroanalytical Chemistry, vol. 379, no. 1-2, pp. 49–61, 1994.

W. Holak and J. J. Specchio, “Determination of selenium in food supplements by differential-pulse cathodic stripping voltammetry in the presence of added copper,” Analyst, vol. 119, no. 10, pp. 2179–2182, 1994.

R. W. Andrews and D. C. Johnson, “Voltammetric deposition and stripping of selenium(IV) at a rotating gold-disk electrode in 0.1 M perchloric acid,” Analytical Chemistry, vol. 47, no. 2, pp. 294–299, 1975.

T. W. Hamilton, J. Ellis, and T. M. Florence, “Determination of selenium and tellurium in electrolytic copper by anodic stripping voltammetry at a gold film electrode,” Analytica Chimica Acta, vol. 110, no. 1, pp. 87–94, 1979.

R. S. Posey and R. W. Andrews, “Determination of selenium(IV) by anodic stripping voltammetry with an in situ gold-plated rotating glassy carbon disk electrode,” Analytica Chimica Acta, vol. 124, no. 1, pp. 107–112, 1981.

J. Wang and J. Lu, “Ultratrace measurements of selenium by cathodic stripping voltammetry in the presence of rhodium,” Analytica Chimica Acta, vol. 274, no. 2, pp. 219–224, 1993.

T. Yano, D. A. Tryk, K. Hashimoto, and A. Fujishima, “Electrochemical behavior of highly conductive boron-doped diamond electrodes for oxygen reduction in alkaline solution,” Journal of the Electrochemical Society, vol. 145, no. 6, pp. 1870–1876, 1998.

A. Fujishima, Y. Einaga, T. N. Rao, and D. A. Tryk, Eds., Diamond Electrochemistry, Elsevier-BKC, Tokyo, Japan, 2005.

D. Yamada, T. A. Ivandini, M. Komatsu, A. Fujishima, and Y. Einaga, “Anodic stripping voltammetry of inorganic species of As³⁺ and As⁵⁺ at gold-modified boron doped diamond electrodes,” Journal of Electroanalytical Chemistry, vol. 615, no. 2, pp. 145–153, 2008.

S. Hrapovic, Y. Liu, and J. H. T. Luong, “Reusable platinum nanoparticle modified boron doped diamond microelectrodes for oxidative determination of arsenite,” Analytical Chemistry, vol. 79, no. 2, pp. 500–507, 2007.